#------------------------------------------------------------------------------
#$Date: 2016-03-26 21:37:51 +0200 (Sat, 26 Mar 2016) $
#$Revision: 180479 $
#$URL: svn://www.crystallography.net/cod/cif/7/21/48/7214849.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_7214849
loop_
_publ_author_name
'Zhu, Zhaojie'
'Zeng, Huiyi'
'Li, Jianfu'
'You, Zhenyu'
'Wang, Yan'
'Huang, Zixiang'
'Tu, Chaoyang'
_publ_section_title
;
 Growth, structure and spectral properties of a novel crystal CaErAlO4 for
 2.7 μm lasers
;
_journal_issue                   21
_journal_name_full               CrystEngComm
_journal_page_first              7423
_journal_paper_doi               10.1039/c2ce26013a
_journal_volume                  14
_journal_year                    2012
_chemical_formula_sum            'Al Ca Er O4'
_chemical_formula_weight         298.32
_chemical_name_systematic
;
?
;
_space_group_IT_number           139
_symmetry_cell_setting           tetragonal
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   3.6420(3)
_cell_length_b                   3.6420(3)
_cell_length_c                   11.814(2)
_cell_measurement_reflns_used    253
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      40.4931
_cell_measurement_theta_min      3.4422
_cell_volume                     156.70(3)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.19 (release 27-10-2011 CrysAlis171 .NET)
(compiled Oct 27 2011,15:02:11)
;
_computing_data_collection
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.19 (release 27-10-2011 CrysAlis171 .NET)
(compiled Oct 27 2011,15:02:11)
;
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.19 (release 27-10-2011 CrysAlis171 .NET)
(compiled Oct 27 2011,15:02:11)
;
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_detector_area_resol_mean 16.2083
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device_type  'Xcalibur, Eos'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'Enhance (Mo) X-ray Source'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0347
_diffrn_reflns_av_sigmaI/netI    0.0450
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -3
_diffrn_reflns_limit_k_max       4
_diffrn_reflns_limit_k_min       -4
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            445
_diffrn_reflns_theta_full        40.59
_diffrn_reflns_theta_max         40.59
_diffrn_reflns_theta_min         3.45
_exptl_absorpt_coefficient_mu    28.525
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.57961
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.35.19 (release 27-10-2011 CrysAlis171 .NET)
(compiled Oct 27 2011,15:02:11)
Empirical absorption correction using spherical harmonics,
implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            brown
_exptl_crystal_density_diffrn    6.323
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       prism
_exptl_crystal_F_000             266
_exptl_crystal_size_max          0.15
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.05
_refine_diff_density_max         2.286
_refine_diff_density_min         -2.502
_refine_diff_density_rms         0.468
_refine_ls_extinction_coef       0.110(8)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.093
_refine_ls_matrix_type           full
_refine_ls_number_parameters     13
_refine_ls_number_reflns         183
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.093
_refine_ls_R_factor_all          0.0313
_refine_ls_R_factor_gt           0.0278
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0271P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0596
_refine_ls_wR_factor_ref         0.0611
_reflns_number_gt                163
_reflns_number_total             183
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            c2ce26013a.txt
_cod_data_source_block           a1
_cod_database_code               7214849
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, -y, z'
'-y, x, z'
'y, -x, z'
'-x, y, -z'
'x, -y, -z'
'y, x, -z'
'-y, -x, -z'
'x+1/2, y+1/2, z+1/2'
'-x+1/2, -y+1/2, z+1/2'
'-y+1/2, x+1/2, z+1/2'
'y+1/2, -x+1/2, z+1/2'
'-x+1/2, y+1/2, -z+1/2'
'x+1/2, -y+1/2, -z+1/2'
'y+1/2, x+1/2, -z+1/2'
'-y+1/2, -x+1/2, -z+1/2'
'-x, -y, -z'
'x, y, -z'
'y, -x, -z'
'-y, x, -z'
'x, -y, z'
'-x, y, z'
'-y, -x, z'
'y, x, z'
'-x+1/2, -y+1/2, -z+1/2'
'x+1/2, y+1/2, -z+1/2'
'y+1/2, -x+1/2, -z+1/2'
'-y+1/2, x+1/2, -z+1/2'
'x+1/2, -y+1/2, z+1/2'
'-x+1/2, y+1/2, z+1/2'
'-y+1/2, -x+1/2, z+1/2'
'y+1/2, x+1/2, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Er Er 0.0000 0.0000 0.35840(5) 0.0048(2) Uani 0.50 8 d SP
Ca Ca 0.0000 0.0000 0.35840(5) 0.0048(2) Uani 0.50 8 d SP
Al Al 0.0000 0.0000 0.0000 0.0033(6) Uani 1 16 d S
O1 O 0.0000 0.5000 0.0000 0.0073(11) Uani 1 8 d S
O2 O 0.0000 0.0000 0.1689(6) 0.0160(15) Uani 1 8 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Al Al 0.0645 0.0514 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Er Er -0.2586 4.9576 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O2 Er O1 132.571(11) . 11
O2 Er O1 132.571(11) . 9_545
O1 Er O1 62.764(12) 11 9_545
O2 Er O1 132.571(11) . 11_545
O1 Er O1 94.86(2) 11 11_545
O1 Er O1 62.764(12) 9_545 11_545
O2 Er O1 132.571(11) . 9_445
O1 Er O1 62.764(12) 11 9_445
O1 Er O1 94.86(2) 9_545 9_445
O1 Er O1 62.764(12) 11_545 9_445
O2 Er O2 82.86(16) . 25_445
O1 Er O2 126.93(13) 11 25_445
O1 Er O2 126.93(13) 9_545 25_445
O1 Er O2 64.37(13) 11_545 25_445
O1 Er O2 64.37(13) 9_445 25_445
O2 Er O2 82.86(17) . 25
O1 Er O2 64.37(13) 11 25
O1 Er O2 64.37(13) 9_545 25
O1 Er O2 126.93(13) 11_545 25
O1 Er O2 126.93(13) 9_445 25
O2 Er O2 165.7(3) 25_445 25
O2 Er O2 82.86(16) . 25_455
O1 Er O2 64.37(13) 11 25_455
O1 Er O2 126.93(13) 9_545 25_455
O1 Er O2 126.93(13) 11_545 25_455
O1 Er O2 64.37(13) 9_445 25_455
O2 Er O2 89.11(4) 25_445 25_455
O2 Er O2 89.11(4) 25 25_455
O2 Er O2 82.86(16) . 25_545
O1 Er O2 126.93(13) 11 25_545
O1 Er O2 64.37(13) 9_545 25_545
O1 Er O2 64.37(13) 11_545 25_545
O1 Er O2 126.93(13) 9_445 25_545
O2 Er O2 89.11(4) 25_445 25_545
O2 Er O2 89.11(4) 25 25_545
O2 Er O2 165.7(3) 25_455 25_545
O2 Er Al 123.006(10) . 9
O1 Er Al 36.369(5) 11 9
O1 Er Al 36.369(5) 9_545 9
O1 Er Al 93.910(17) 11_545 9
O1 Er Al 93.910(17) 9_445 9
O2 Er Al 154.14(17) 25_445 9
O2 Er Al 40.15(16) 25 9
O2 Er Al 93.88(9) 25_455 9
O2 Er Al 93.88(9) 25_545 9
O2 Er Al 123.006(10) . 9_445
O1 Er Al 93.910(17) 11 9_445
O1 Er Al 93.910(17) 9_545 9_445
O1 Er Al 36.369(5) 11_545 9_445
O1 Er Al 36.369(5) 9_445 9_445
O2 Er Al 40.15(16) 25_445 9_445
O2 Er Al 154.14(17) 25 9_445
O2 Er Al 93.88(9) 25_455 9_445
O2 Er Al 93.88(9) 25_545 9_445
Al Er Al 113.99(2) 9 9_445
O2 Er Al 123.006(10) . 9_455
O1 Er Al 36.369(5) 11 9_455
O1 Er Al 93.910(17) 9_545 9_455
O1 Er Al 93.910(17) 11_545 9_455
O1 Er Al 36.369(5) 9_445 9_455
O2 Er Al 93.88(9) 25_445 9_455
O2 Er Al 93.88(9) 25 9_455
O2 Er Al 40.15(16) 25_455 9_455
O2 Er Al 154.14(17) 25_545 9_455
Al Er Al 72.739(9) 9 9_455
Al Er Al 72.739(9) 9_445 9_455
O1 Al O1 90.0 3_655 .
O1 Al O1 180.0 3_655 3
O1 Al O1 90.0 . 3
O1 Al O1 90.0 3_655 1_545
O1 Al O1 180.0 . 1_545
O1 Al O1 90.0 3 1_545
O1 Al O2 90.0 3_655 17
O1 Al O2 90.0 . 17
O1 Al O2 90.0 3 17
O1 Al O2 90.0 1_545 17
O1 Al O2 90.0 3_655 .
O1 Al O2 90.0 . .
O1 Al O2 90.0 3 .
O1 Al O2 90.0 1_545 .
O2 Al O2 180.0 17 .
O1 Al Er 126.369(5) 3_655 9_444
O1 Al Er 126.369(5) . 9_444
O1 Al Er 53.631(5) 3 9_444
O1 Al Er 53.631(5) 1_545 9_444
O2 Al Er 56.994(10) 17 9_444
O2 Al Er 123.006(10) . 9_444
O1 Al Ca 53.631(5) 3_655 25
O1 Al Ca 53.631(5) . 25
O1 Al Ca 126.369(5) 3 25
O1 Al Ca 126.369(5) 1_545 25
O2 Al Ca 123.006(10) 17 25
O2 Al Ca 56.994(10) . 25
Er Al Ca 180.000(17) 9_444 25
O1 Al Ca 126.369(5) 3_655 9_444
O1 Al Ca 126.369(5) . 9_444
O1 Al Ca 53.631(5) 3 9_444
O1 Al Ca 53.631(5) 1_545 9_444
O2 Al Ca 56.994(10) 17 9_444
O2 Al Ca 123.006(10) . 9_444
Er Al Ca 0.000(17) 9_444 9_444
Ca Al Ca 180.000(17) 25 9_444
O1 Al Er 53.631(5) 3_655 25
O1 Al Er 53.631(5) . 25
O1 Al Er 126.369(5) 3 25
O1 Al Er 126.369(5) 1_545 25
O2 Al Er 123.006(10) 17 25
O2 Al Er 56.994(10) . 25
Er Al Er 180.000(17) 9_444 25
Ca Al Er 0.000(17) 25 25
Ca Al Er 180.000(17) 9_444 25
O1 Al Er 53.631(5) 3_655 9_554
O1 Al Er 53.631(5) . 9_554
O1 Al Er 126.369(5) 3 9_554
O1 Al Er 126.369(5) 1_545 9_554
O2 Al Er 56.994(10) 17 9_554
O2 Al Er 123.006(10) . 9_554
Er Al Er 113.99(2) 9_444 9_554
Ca Al Er 66.01(2) 25 9_554
Ca Al Er 113.99(2) 9_444 9_554
Er Al Er 66.01(2) 25 9_554
O1 Al Er 126.369(5) 3_655 25_445
O1 Al Er 126.369(5) . 25_445
O1 Al Er 53.631(5) 3 25_445
O1 Al Er 53.631(5) 1_545 25_445
O2 Al Er 123.006(10) 17 25_445
O2 Al Er 56.994(10) . 25_445
Er Al Er 66.01(2) 9_444 25_445
Ca Al Er 113.99(2) 25 25_445
Ca Al Er 66.01(2) 9_444 25_445
Er Al Er 113.99(2) 25 25_445
Er Al Er 180.000(17) 9_554 25_445
Al O1 Al 180.0 1_565 .
Al O1 Er 90.0 1_565 9_454
Al O1 Er 90.0 . 9_454
Al O1 Ca 90.0 1_565 25
Al O1 Ca 90.0 . 25
Er O1 Ca 180.000(19) 9_454 25
Al O1 Ca 90.0 1_565 9_454
Al O1 Ca 90.0 . 9_454
Er O1 Ca 0.000(19) 9_454 9_454
Ca O1 Ca 180.0 25 9_454
Al O1 Er 90.0 1_565 25
Al O1 Er 90.0 . 25
Er O1 Er 180.000(19) 9_454 25
Ca O1 Er 0.000(19) 25 25
Ca O1 Er 180.000(19) 9_454 25
Al O1 Er 90.0 1_565 9_554
Al O1 Er 90.0 . 9_554
Er O1 Er 94.86(2) 9_454 9_554
Ca O1 Er 85.14(2) 25 9_554
Ca O1 Er 94.86(2) 9_454 9_554
Er O1 Er 85.14(2) 25 9_554
Al O1 Ca 90.0 1_565 9_554
Al O1 Ca 90.0 . 9_554
Er O1 Ca 94.86(2) 9_454 9_554
Ca O1 Ca 85.14(2) 25 9_554
Ca O1 Ca 94.86(2) 9_454 9_554
Er O1 Ca 85.14(2) 25 9_554
Er O1 Ca 0.000(19) 9_554 9_554
Al O1 Ca 90.0 1_565 25_455
Al O1 Ca 90.0 . 25_455
Er O1 Ca 85.14(2) 9_454 25_455
Ca O1 Ca 94.86(2) 25 25_455
Ca O1 Ca 85.14(2) 9_454 25_455
Er O1 Ca 94.86(2) 25 25_455
Er O1 Ca 180.0 9_554 25_455
Ca O1 Ca 180.0 9_554 25_455
Al O1 Er 90.0 1_565 25_455
Al O1 Er 90.0 . 25_455
Er O1 Er 85.14(2) 9_454 25_455
Ca O1 Er 94.86(2) 25 25_455
Ca O1 Er 85.14(2) 9_454 25_455
Er O1 Er 94.86(2) 25 25_455
Er O1 Er 180.0 9_554 25_455
Ca O1 Er 180.0 9_554 25_455
Ca O1 Er 0.0 25_455 25_455
Al O2 Er 180.0 . .
Al O2 Ca 82.86(16) . 25_445
Er O2 Ca 97.14(16) . 25_445
Al O2 Er 82.86(16) . 25_445
Er O2 Er 97.14(16) . 25_445
Ca O2 Er 0.00(2) 25_445 25_445
Al O2 Ca 82.86(16) . 25
Er O2 Ca 97.14(16) . 25
Ca O2 Ca 165.7(3) 25_445 25
Er O2 Ca 165.7(3) 25_445 25
Al O2 Er 82.86(16) . 25
Er O2 Er 97.14(16) . 25
Ca O2 Er 165.7(3) 25_445 25
Er O2 Er 165.7(3) 25_445 25
Ca O2 Er 0.00(2) 25 25
Al O2 Er 82.86(16) . 25_455
Er O2 Er 97.14(16) . 25_455
Ca O2 Er 89.11(4) 25_445 25_455
Er O2 Er 89.11(4) 25_445 25_455
Ca O2 Er 89.11(4) 25 25_455
Er O2 Er 89.11(4) 25 25_455
Al O2 Er 82.86(16) . 25_545
Er O2 Er 97.14(16) . 25_545
Ca O2 Er 89.11(4) 25_445 25_545
Er O2 Er 89.11(4) 25_445 25_545
Ca O2 Er 89.11(4) 25 25_545
Er O2 Er 89.11(4) 25 25_545
Er O2 Er 165.7(3) 25_455 25_545
Al O2 Ca 82.86(16) . 25_545
Er O2 Ca 97.14(16) . 25_545
Ca O2 Ca 89.11(4) 25_445 25_545
Er O2 Ca 89.11(4) 25_445 25_545
Ca O2 Ca 89.11(4) 25 25_545
Er O2 Ca 89.11(4) 25 25_545
Er O2 Ca 165.7(3) 25_455 25_545
Er O2 Ca 0.00(2) 25_545 25_545
Al O2 Ca 82.86(16) . 25_455
Er O2 Ca 97.14(16) . 25_455
Ca O2 Ca 89.11(4) 25_445 25_455
Er O2 Ca 89.11(4) 25_445 25_455
Ca O2 Ca 89.11(4) 25 25_455
Er O2 Ca 89.11(4) 25 25_455
Er O2 Ca 0.00(2) 25_455 25_455
Er O2 Ca 165.7(3) 25_545 25_455
Ca O2 Ca 165.7(3) 25_545 25_455
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Er O2 2.238(7) .
Er O1 2.4727(4) 11
Er O1 2.4727(4) 9_545
Er O1 2.4727(4) 11_545
Er O1 2.4727(4) 9_445
Er O2 2.5954(10) 25_445
Er O2 2.5954(10) 25
Er O2 2.5954(10) 25_455
Er O2 2.5954(10) 25_545
Er Al 3.0709(4) 9
Er Al 3.0709(4) 9_445
Er Al 3.0709(4) 9_455
Al O1 1.82100(15) 3_655
Al O1 1.82100(15) .
Al O1 1.82100(15) 3
Al O1 1.82100(15) 1_545
Al O2 1.996(7) 17
Al O2 1.996(7) .
Al Er 3.0709(4) 9_444
Al Ca 3.0709(4) 25
Al Ca 3.0709(4) 9_444
Al Er 3.0709(4) 25
Al Er 3.0709(4) 9_554
Al Er 3.0709(4) 25_445
O1 Al 1.82100(15) 1_565
O1 Er 2.4727(4) 9_454
O1 Ca 2.4727(4) 25
O1 Ca 2.4727(4) 9_454
O1 Er 2.4727(4) 25
O1 Er 2.4727(4) 9_554
O1 Ca 2.4727(4) 9_554
O1 Ca 2.4727(4) 25_455
O1 Er 2.4727(4) 25_455
O2 Ca 2.5954(10) 25_445
O2 Er 2.5954(10) 25_445
O2 Ca 2.5954(10) 25
O2 Er 2.5954(10) 25
O2 Er 2.5954(10) 25_455
O2 Er 2.5954(10) 25_545
O2 Ca 2.5954(10) 25_545
O2 Ca 2.5954(10) 25_455
